Cadmium telluride

Short description: Semiconductor chemical compound used in solar cells

Cadmium telluride

Names
Other names

Irtran-6

Identifiers

CAS Number

* 1306-25-8 Y

3D model (JSmol)

* monomer: Interactive image
* crystal form: Interactive image

ChemSpider |

* 82622 Y

EC Number |

* 215-149-9

PubChem CID

* 91501

RTECS number |

* EV3330000

UNII |

* STG188WO13

InChI

* InChI=1S/Cd.Te Y

Key: RPPBZEBXAAZZJH-UHFFFAOYSA-N Y

* InChI=1/Cd.Te/rCdTe/c1-2

Key: RPPBZEBXAAZZJH-UEZHWRJLAD

SMILES

* monomer: [Cd]=[Te]

* crystal form: [TeH+2]12[CdH2-2][TeH+2]3[CdH2-2][TeH+2]([CdH-2]14)[CdH-2]1[Te+2]5([CdH-2]38)[Cd-2]26[TeH+2]2[CdH-2]([Te+2]4)[TeH+2]1[CdH2-2][TeH+2]3[CdH-2]2[Te+2][CdH-2]([TeH+2]6[CdH-2]([TeH+2])[TeH+2]68)[TeH+2]([CdH2-2]6)[CdH-2]35

Properties

Chemical formula

| CdTe
Molar mass | 240.01 g/mol
Density | 5.85 g·cm−3[1]
Melting point |  1,041 °C (1,906 °F; 1,314 K)[2]
Boiling point |  1,050 °C (1,920 °F; 1,320 K)

Solubility in water

| insoluble
Solubility in other solvents  | insoluble
Band gap | 1.5 eV (@300 K, direct)
Thermal conductivity | 6.2 W·m/m2·K at 293 K

Refractive index (nD)

| 2.67 (@10 µm)
Structure

Crystal structure

| Zinc blende

Space group

| F43m

Lattice constant

a = 0.648 nm

Thermochemistry

Heat capacity (C)

| 210 J/kg·K at 293 K
Hazards
GHS pictograms |
GHS Signal word | Warning

GHS hazard statements

| H302, H312, H332, H410, H411

GHS precautionary statements

| P261, P264, P270, P271, P273, P280, P301+312, P302+352, P304+312, P304+340, P312, P322, P330, P363, P391, P501
NIOSH (US health exposure limits):

PEL (Permissible)

| [1910.1027] TWA 0.005 mg/m3 (as Cd)[3]

REL (Recommended)

| Ca[3]

IDLH (Immediate danger)

| Ca [9 mg/m3 (as Cd)][3]
Related compounds

Other anions

| Cadmium oxide
Cadmium sulfide
Cadmium selenide

Other cations

| Zinc telluride
Mercury telluride

Except where otherwise noted, data are given for materials in their standard state (at 25 °C [77 °F], 100 kPa).

Y verify (what is YN ?)
Infobox references

Cadmium telluride (CdTe) is a stable crystalline compound formed from cadmium and tellurium. It is mainly used as the semiconducting material in cadmium telluride photovoltaics and an infrared optical window. It is usually sandwiched with cadmium sulfide to form a p–n junction solar PV cell.

## Contents

* 1 Applications
* 2 Physical properties
* 2.1 Optical and electronic properties
* 3 Chemical properties
* 4 Toxicology assessment
* 5 Availability
* 6 See also
* 7 References
* 8 External links

## Applications

CdTe is used to make thin film solar cells, accounting for about 8% of all solar cells installed in 2011.[4] They are among the lowest-cost types of solar cell,[5] although a comparison of total installed cost depends on installation size and many other factors, and has changed rapidly from year to year. The CdTe solar cell market is dominated by First Solar. In 2011, around 2 GWp of CdTe solar cells were produced;[4] For more details and discussion see cadmium telluride photovoltaics.

CdTe can be alloyed with mercury to make a versatile infrared detector material (HgCdTe). CdTe alloyed with a small amount of zinc makes an excellent solid-state X-ray and gamma ray detector (CdZnTe).

CdTe is used as an infrared optical material for optical windows and lenses and is proven to provide a good performance across a wide range of temperatures.[6] An early form of CdTe for IR use was marketed under the trademarked name of Irtran-6, but this is obsolete.

CdTe is also applied for electro-optic modulators. It has the greatest electro-optic coefficient of the linear electro-optic effect among II-VI compound crystals (r41=r52=r63=6.8×10−12 m/V).

CdTe doped with chlorine is used as a radiation detector for x-rays, gamma rays, beta particles and alpha particles. CdTe can operate at room temperature allowing the construction of compact detectors for a wide variety of applications in nuclear spectroscopy.[7] The properties that make CdTe superior for the realization of high performance gamma- and x-ray detectors are high atomic number, large bandgap and high electron mobility ~1100 cm2/V·s, which result in high intrinsic μτ (mobility-lifetime) product and therefore high degree of charge collection and excellent spectral resolution.[8] Due to the poor charge transport properties of holes, ~100 cm2/V·s, single-carrier-sensing detector geometries are used to produce high resolution spectroscopy; these include coplanar grids, Frisch-collar detectors and small pixel detectors.

## Physical properties

* Thermal expansion coefficient: 5.9×10−6/K at 293 K[9]
* Young's modulus: 52 GPa
* Poisson ratio: 0.41

### Optical and electronic properties

Fluorescence spectra of colloidal CdTe quantum dots of various sizes, increasing approximately from 2 to 20 nm from left to right. The blue shift of fluorescence is due to quantum confinement.

Bulk CdTe is transparent in the infrared, from close to its band gap energy (1.5 eV at 300 K,[10] which corresponds to infrared wavelength of about 830 nm) out to wavelengths greater than 20 µm; correspondingly, CdTe is fluorescent at 790 nm. As the size of CdTe crystals are reduced to a few nanometers or less, thus making them CdTe quantum dots, the fluorescence peak shifts through the visible range into the ultraviolet.

## Chemical properties

CdTe is insoluble in water.[11] CdTe has a high melting point of 1041 °C with evaporation starting at 1050 °C.[12] CdTe has a vapor pressure of zero at ambient temperatures. CdTe is more stable than its parent compounds cadmium and tellurium and most other Cd compounds, due to its high melting point and insolubility.[13]

Cadmium telluride is commercially available as a powder, or as crystals. It can be made into nanocrystals.

## Toxicology assessment

The compound CdTe has different qualities than the two elements, cadmium and tellurium, taken separately. CdTe has low acute inhalation, oral, and aquatic toxicity, and is negative in the Ames mutagenicity test. Based on notification of these results to the European Chemicals Agency (ECHA), CdTe is no longer classified as harmful if ingested nor harmful in contact with skin, and the toxicity classification to aquatic life has been reduced.[14] Once properly and securely captured and encapsulated, CdTe used in manufacturing processes may be rendered harmless. Current CdTe modules pass the U.S. EPA’s Toxicity Characteristic Leaching Procedure (TCLP) test, designed to assess the potential for long-term leaching of products disposed in landfills.[15]

A document hosted by the U.S. National Institutes of Health[16] dated 2003 discloses that:

> Brookhaven National Laboratory (BNL) and the U.S. Department of Energy (DOE) are nominating Cadmium Telluride (CdTe) for inclusion in the National Toxicology Program (NTP). This nomination is strongly supported by the National Renewable Energy Laboratory (NREL) and First Solar Inc. The material has the potential for widespread applications in photovoltaic energy generation that will involve extensive human interfaces. Hence, we consider that a definitive toxicological study of the effects of long-term exposure to CdTe is a necessity.

According to the classification provided by companies to the European Chemicals Agency (ECHA) in REACH registrations, it is still harmful to aquatic life with long lasting effects.

Additionally, the classification provided by companies to ECHA notifications classifies it as very toxic to aquatic life with long lasting effects, very toxic to aquatic life, harmful if inhaled or swallowed and is harmful in contact with skin.[17]

## Availability

At the present time, the prices of the raw materials cadmium and tellurium are a negligible proportion of the cost of CdTe solar cells and other CdTe devices. However, tellurium is a relatively rare element (1–5 parts per billion in the Earth's crust; see Abundances of the elements (data page)). Through improved material efficiency and increased PV recycling systems, the CdTe PV industry has the potential to fully rely on tellurium from recycled end-of-life modules by 2038.[18] See Cadmium telluride photovoltaics for more information. Another study shows that CdTe PV recycling will add a significant secondary resource of Te which, in conjunction with improved material utilization, will enable a cumulative capacity of about 2 TW by 2050 and 10 TW by the end of the century.[19]

## See also

* Cadmium selenide
* Cadmium telluride photovoltaics
* Cadmium zinc telluride
* First Solar
* Mercury telluride
* Mercury(II) cadmium(II) telluride
* Zinc telluride

## References

1. ↑ Peter Capper (1994). Properties of Narrow Gap Cadmium-Based Compounds. IET. pp. 39–. ISBN 978-0-85296-880-2. https://books.google.com/books?id=WAhC3hGYQ7UC&pg=PA39. Retrieved 1 June 2012.
2. ↑ "Nomination of Cadmium Telluride to the National Toxicology Program". United States Department of Health and Human Services. https://ntp.niehs.nih.gov/ntp/htdocs/chem_background/exsumpdf/cdte_508.pdf.
3. ↑ 3.0 3.1 3.2 NIOSH Pocket Guide to Chemical Hazards. "#0087". National Institute for Occupational Safety and Health (NIOSH). https://www.cdc.gov/niosh/npg/npgd0087.html.
4. ↑ 4.0 4.1 "Photovoltaics report". http://www.ise.fraunhofer.de/de/downloads/pdf-files/aktuelles/photovoltaics-report.pdf.
5. ↑ "Introduction". Chalcogenide Photovoltaics. 2011. pp. 1–8. doi:10.1002/9783527633708.ch1. ISBN 9783527633708.
6. ↑ "Cadmium Telluride". http://www.reading.ac.uk/infrared/library/infraredmaterials.
7. ↑ P. Capper (1994). Properties of Narrow-Gap Cadmium-Based Compounds. London, UK: INSPEC, IEE. ISBN 978-0-85296-880-2.
8. ↑ Veale, M. C.; Kalliopuska, J.; Pohjonen, H.; Andersson, H.; Nenonen, S.; Seller, P.; Wilson, M. D. (2012). "Characterization of M-π-n CdTe pixel detectors coupled to HEXITEC readout chip". Journal of Instrumentation 7 (1): C01035. doi:10.1088/1748-0221/7/01/C01035. Bibcode: 2012JInst...7C1035V.
9. ↑ Palmer, D W (March 2008). "Properties of II-VI Compound Semiconductors". Semiconductors-Information. http://www.semiconductors.co.uk/propiivi5410.htm.
10. ↑ Fonthal, G. (2000). "Temperature dependence of the band gap energy of crystalline CdTe". J. Phys. Chem. Solids 61 (4): 579–583. doi:10.1016/s0022-3697(99)00254-1. Bibcode: 2000JPCS...61..579F.
11. ↑ Solubility is below 0.1mg/L which equals a classification as insoluble- reference, "ECHA Substance Registration"[1]
12. ↑ "Cadmium Telluride". http://apps.echa.europa.eu/registered/data/dossiers/DISS-dffb4072-e283-47ae-e044-00144f67d031/DISS-dffb4072-e283-47ae-e044-00144f67d031_DISS-dffb4072-e283-47ae-e044-00144f67d031.html.
13. ↑ S. Kaczmar (2011). "Evaluating the read-across approach on CdTe toxicity for CdTe photovoltaics". ftp://ftp.co.imperial.ca.us/icpds/eir/campo-verde-solar/final/evaluating-toxicity.pdf. [yes|permanent dead link|dead link}}]
14. ↑ "Scientific Comment of Fraunhofer to Life Cycle Assessement [sic] of CdTe Photovoltaics". Fraunhofer Center for Silicon Photovoltaics CSP. http://www.csp.fraunhofer.de/presse-und-veranstaltungen/details/id/47/.
15. ↑ "CdTe PV: Real and Perceived EHS Risks". National Renewable Energy Laboratory. 2003. http://www.nrel.gov/docs/fy03osti/33561.pdf.
16. ↑ ﻿Nomination of Cadmium Telluride to the National Toxicology Program﻿ (Report). United States Department of Health and Human Services. 2003-04-11. https://ntp.niehs.nih.gov/ntp/htdocs/chem_background/exsumpdf/cdte_508.pdf.
17. ↑ "Cadmium telluride - Brief Profile - ECHA". European Chemicals Agency. 2020. https://echa.europa.eu/brief-profile/-/briefprofile/100.013.773.
18. ↑ M. Marwede; A. Reller (2012). "Future recycling flows of tellurium from cadmium telluride photovoltaic waste". Resources, Conservation and Recycling 69: 35–49. doi:10.1016/j.resconrec.2012.09.003. https://depositonce.tu-berlin.de/bitstream/11303/7375/3/2012_marwede_et-al.pdf.
19. ↑ Fthenakis, V.M. (2012). "Sustainability metrics for extending thin-film photovoltaics to terawatt levels". MRS Bulletin 37 (4): 425–430. doi:10.1557/mrs.2012.50.

## External links

* CdTe page on the web-site of the Institute of Solid State Physics of the Russian Academy of Sciences (html)
* Optical properties University of Reading, Infrared Multilayer Laboratory
* CdTe: single crystals, grown by HPVB and HPVZM techniques; windows, substrates, electrooptical modulators. Infrared transmittance spectrum. MSDS.
* National Pollutant Inventory – Cadmium and compounds
* MSDS at ISP optics.com (doc)
* MDSD at espimetals.com (pdf)
* Material Safety data Sheet on isp optics web site (MS Word doc)

* v
* t
* e

Cadmium compounds

Cadmium(I)|

* Cd2(AlCl4)2

Cadmium(II)|

* Cd(BF4)2
* CdF2
* CdCl2
* CdBr2
* CdI2
* Cd(CN)2
* CdH2
* CdO
* CdS
* CdSe
* CdTe
* Cd(OH)2
* Cd(NO3)2
* CdSO4
* CdWO4
* Cd3As2
* CsCdCl3
* CsCdBr3

0.00

(0 votes)

Original source: https://en.wikipedia.org/wiki/Cadmium telluride. Read more

|

Retrieved from "https://handwiki.org/wiki/index.php?title=Chemistry:Cadmium_telluride&oldid=247196"
*[CID]: Compound ID
*[H302]: Harmful if swallowed
*[H312]: Harmful in contact with skin
*[H332]: Harmful if inhaled
*[H410]: Very toxic to aquatic life with long lasting effects
*[H411]: Toxic to aquatic life with long lasting effects
*[P261]: Avoid breathing dust/fume/gas/mist/vapours/spray
*[P264]: Wash … thoroughly after handling
*[P270]: Do not eat, drink or smoke when using this product
*[P271]: Use only outdoors or in a well-ventilated area
*[P273]: Avoid release to the environment
*[P280]: Wear protective gloves/protective clothing/eye protection/face protection
*[P301+312]: IF SWALLOWED: Call a POISON CENTER or doctor/physician if you feel unwell
*[P302+352]: IF ON SKIN: Wash with soap and water
*[P304+312]: IF INHALED: Call a POISON CENTER or doctor/physician if you feel unwell
*[P304+340]: IF INHALED: Remove victim to fresh air and keep at rest in a position comfortable for breathing
*[P312]: Call a POISON CENTER or doctor/physician if you feel unwell
*[P322]: Specific measures (see … on this label)
*[P330]: Rinse mouth
*[P363]: Wash contaminated clothing before reuse
*[P391]: Collect spillage
*[P501]: Dispose of contents/container to …
*[v]: View this template
*[t]: Discuss this template
*[e]: Edit this template